Spin crossover iron(II) coordination polymer chains: syntheses, structures, and magnetic characterizations of [Fe(aqin)2(μ2-M(CN)4)] (M = Ni(II), Pt(II), aqin = quinolin-8-amine).
Setifi, Fatima; Milin, Eric; Charles, Catherine; Thétiot, Franck; Triki, Smail; Gómez-García, Carlos J; Inorganic chemistry 53 (2014) 97–104; doi:10.1021/ic401721x

data_4337446
_publ_section_title
;
 Spin crossover iron(II) coordination polymer chains: syntheses,
 structures, and magnetic characterizations of [Fe(aqin)2(\m2-M(CN)4)] (M
 = Ni(II), Pt(II), aqin = quinolin-8-amine).
;
_journal_issue                   1
_journal_name_full               'Inorganic chemistry'
_journal_page_first              97
_journal_page_last               104
_journal_paper_doi               10.1021/ic401721x
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'C22 H16 Fe N8 Pt'
_chemical_formula_weight         643.37
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4
_audit_creation_date             2013-01-25T16:54:02-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 101.670(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.3073(3)
_cell_length_b                   12.1228(4)
_cell_length_c                   9.9073(3)
_cell_measurement_reflns_used    4776
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      31.4422
_cell_measurement_theta_min      3.2051
_cell_volume                     1094.74(6)
_computing_cell_refinement
;
        CrysAlis RED, Oxford Diffraction Ltd.,
        Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
        (compiled Nov  6 2009,16:24:50)
;
_computing_data_collection
;
        CrysAlis CCD, Oxford Diffraction Ltd.,
        Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
        (compiled Nov  6 2009,16:24:50)
;
_computing_data_reduction
;
        CrysAlis RED, Oxford Diffraction Ltd.,
        Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
        (compiled Nov  6 2009,16:24:50)
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 8.3622
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Xcalibur 2 CCD Oxford Diffraction'
_diffrn_measurement_method       'omega scan'
_diffrn_orient_matrix_UB_11      0.0066859494
_diffrn_orient_matrix_UB_12      -0.0270651208
_diffrn_orient_matrix_UB_13      0.0686448041
_diffrn_orient_matrix_UB_21      0.0188081986
_diffrn_orient_matrix_UB_22      -0.0493630434
_diffrn_orient_matrix_UB_23      -0.031781751
_diffrn_orient_matrix_UB_31      0.0703823735
_diffrn_orient_matrix_UB_32      0.0157992687
_diffrn_orient_matrix_UB_33      0.0183838832
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.033
_diffrn_reflns_av_unetI/netI     0.0354
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            10604
_diffrn_reflns_theta_full        29.99
_diffrn_reflns_theta_max         29.99
_diffrn_reflns_theta_min         3.21
_exptl_absorpt_coefficient_mu    7.072
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.62684
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
        CrysAlis RED, Oxford Diffraction Ltd.,
        Version 1.171.33.52 (release 06-11-2009 CrysAlis171 .NET)
        (compiled Nov  6 2009,16:24:50)
        Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    1.952
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             616
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.89
_refine_diff_density_min         -0.351
_refine_diff_density_rms         0.114
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.973
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     148
_refine_ls_number_reflns         3174
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.973
_refine_ls_R_factor_all          0.0493
_refine_ls_R_factor_gt           0.0226
_refine_ls_shift/su_max          0
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0246P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0494
_refine_ls_wR_factor_ref         0.0539
_reflns_number_gt                2017
_reflns_number_total             3174
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            ic401721x_si_003.cif
_cod_data_source_block           Fe(amq)2(Pt(CN)4-293K
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      P21/c
_cod_database_code               4337446